https://doi.org/10.1038/s41467-021-21911-z OPEN On-surface preparation of coordinated lanthanide-transition-metal clusters
Jing Liu 1,2, Jie Li1,3, Zhen Xu1, Xiong Zhou4, Qiang Xue1, Tianhao Wu1, Mingjun Zhong1, Ruoning Li1, Rong Sun4, ✉ Ziyong Shen1, Hao Tang5, Song Gao 2,4,6, Bingwu Wang4, Shimin Hou1,3 & Yongfeng Wang 1,2,6
The study of lanthanide (Ln)-transition-metal (TM) heterometallic clusters which play key roles in various high-tech applications is a rapid growing ﬁeld of research. Despite the
1234567890():,; achievement of numerous Ln-TM cluster compounds comprising one Ln atom, the synthesis of Ln-TM clusters containing multiple Ln atoms remains challenging. Here, we present the preparation and self-assembly of a series of Au-bridged heterometallic clusters containing multiple cerium (Ce) atoms via on-surface coordination. By employing different pyridine and nitrile ligands, the ordered coordination assemblies of clusters containing 2, 3 and 4 Ce atoms bridged by Au adatoms are achieved on Au(111) and Au(100), as revealed by scanning tunneling microscopy. Density functional theory calculations uncover the indispensable role of the bridging Au adatoms in constructing the multi-Ce-containing clusters by connecting the Ce atoms via unsupported Ce-Au bonds. These ﬁndings demonstrate on-surface coor- dination as an efﬁcient strategy for preparation and organization of the multi-Ln-containing heterometallic clusters.
1 Key Laboratory for the Physics and Chemistry of Nanodevices and Center for Carbon-based Electronics, Department of Electronics, Peking University, Beijing, China. 2 Division of Quantum State of Matter, Beijing Academy of Quantum Information Sciences, Beijing, China. 3 Peking University Information Technology Institute (Tianjin Binhai), Tianjin, China. 4 Beijing National Laboratory of Molecular Science, College of Chemistry and Molecular Engineering, Peking University, Beijing, China. 5 CEMES, UPR CNRS 8011, Toulouse Cedex 4, France. 6 Institute of Spin Science and Technology, South China University of ✉ Technology, Guangzhou, China. email: [email protected]
NATURE COMMUNICATIONS | (2021) 12:1619 | https://doi.org/10.1038/s41467-021-21911-z | www.nature.com/naturecommunications 1 ARTICLE NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-021-21911-z
anthanide (Ln) series comprises lanthanum (La) and the metal–metal bonds. Recently, a series of Ln–organic hybrids have following 14 f-block metal elements from cerium (Ce) to been constructed via on-surface coordination, in which either L 14–24 17 lutetium (Lu). One of the research frontiers devoted to Ln- single Ln atoms or molecule-bridged Ln dimers were engaged materials in recent years is the heterometallic com- identiﬁed as the coordination centers. Meanwhile, the achieve- pounds containing directly bonded Ln and transition-metal (TM) ment of non-lanthanide metallic clusters stabilized by organic atoms. Such Ln–TM heterometallic compounds register various ligands on surfaces were also reported25–30. Nevertheless, the on- potential applications, including high-performance permanent surface preparation of coordination complexes formed by TM- magnets, hydrogen storage materials, luminescent materials, and bridged multi-Ln-containing heterometallic clusters has yet to be catalysts, etc.1–3. Moreover, the direct (or unsupported) realized. metal–metal bonds between f-block and d-block elements in the In this work, we show the preparation of a series of multi-Ce- compounds are of great interest in terms of bonding theory. containing heterometallic clusters in which the Ce atoms are Tremendous effort has been devoted to preparation of coordi- bridged by Au atoms via the unsupported Ce–Au bonds with an nation compounds involving both Ln metals and TMs by wet on-surface coordination strategy. By applying various molecular chemistry, resulting in a number of Ln–TM heterometallic ligands (Fig. 1a), including the pyridines (Py) 1 [1,4-bis(4-pyr- coordination complexes featuring unsupported d–f metal–metal idyl)-benzene], 3 [1,4-bis(4-pyridyl)-biphenyl], and 4 [1,3-bis(4- bonds4–7. Most of these heterometallic compounds possess metal pyridyl)-benzene], and the nitrile (CN) 2 [4,4″-dicyano-1,1′:3′,1″- cores comprising only one Ln atom bonded to one or more TM- terphenyl], Ce–Au heterometallic clusters coordinated by the containing metalloligand(s), whereas formation of Ln–TM clus- organic linkers are obtained on different Au substrates [Au(111) ters involving multiple Ln atoms as coordination centers in the and Au(100)], as revealed by the scanning tunneling microscopy compounds is scarcely reported8. The multi-Ln-containing het- (STM) investigations. The heterometallic clusters containing 2, 3, erometallic clusters are expected to exhibit novel properties and and 4 Ce atoms in which each pair of the nearest-neighboring Ce improved performance owning to the interactions supposed to atoms are bridged by two Au adatoms assemble into ordered one- emerge between the multiple Ln atoms in the clusters such as or two-dimensional (1D or 2D) structures by forming different their magnetic coupling and synergistic effects in catalysis. coordination motifs with the molecular ligands (Fig. 1b), leading Moreover, to include multiple Ln atoms in one Ln–TM cluster to to mono-dispersed domains of the Ce–Au clusters. Density build up larger heterometallic aggregates would also narrow the functional theory (DFT) studies reveal the indispensable role of gap between molecular heterometallic complexes and inter- the bridging Au adatoms in stabilizing the multiple Ce atoms metallic solid-state compounds. Therefore, the exploration of the within one cluster by forming the unsupported Ce–Au bonds preparation of Ln–TM heterometallic clusters containing multiple between them. This work demonstrates on-surface coordination Ln atoms is highly desirable. as an efﬁcient strategy for preparing and organizing TM-bridged The formation of the multi-Ln-containing Ln–TM clusters multi-Ln-containing heterometallic clusters stabilized by unsup- stabilized by unsupported metal–metal bonds requires delicate ported d–f metal–metal bonds. balance among the various metal–metal and metal–ligand inter- actions, whose realization by wet chemistry would be rather Results challenging mainly due to the less controllable reaction condi- Coordination structures involving Ce and pyridine ligand 1 tions in the solvent environment. Fortunately, on-surface coor- formed on Au(111). Deposition of 1 onto the Au(111) substrate dination chemistry has evolved in the past two decades to be an held at room temperature gave rise to a self-assembled structure efﬁcient approach to fabricating a plenty of low-dimensional stabilized by intermolecular hydrogen bonds (Supplementary metal–organic hybrid nanostructures that cannot be achieved by – Fig. 1a). Upon evaporation of Ce atoms onto the 1-precovered Au wet chemistry9 13. In the on-surface coordination systems, the (111) substrate held at room temperature, the formation of a coordination reactions are conﬁned in the 2D plane due to the single-wall honeycomb network (Fig. 2a) was observed. The absorbate–substrate interactions. Moreover, the ultrahigh vacuum hexagonal unit cell of the new structure is highlighted by the (UHV) condition in which the on-surface constructions of white parallelogram in Fig. 2a with a periodicity of 2.6 nm. This coordination structures are usually carried out ensures a solvent- 2D network is distinct from that obtained by the coordination of free reaction environment. Both facts facilitate the controllability 1 with the Au adatoms on Au(111), that is, the 1D molecular of the coordination reactions on surfaces. On-surface coordina- wires in which the molecules are connected by twofold coordi- tion thus provides a potential solution to the preparation of the nation with the Au adatoms (Supplementary Fig. 1b)31. There- multi-Ln-containing Ln–TM clusters stabilized by unsupported fore, it is Ce atoms rather than Au adatoms that are engaged in
N N N N N N NC CN 1342
b α α α Ce α Au
Ligand (L) CeL3 Ce2Au2L4 Ce2Au2L6 Ce3Au4L6 Ce4Au5L8 L = 1, 2, 3, 4 L = 1, 3, 4 L = 2 L = 1, 3 L = 2
Fig. 1 Ligands used and coordination motifs achieved in this work. a Chemical structures of the molecular ligands 1 [1,4-bis(4-pyridyl)-benzene], 2 [4,4″- dicyano-1,1′:3′,1″-terphenyl], 3 [1,4-bis(4-pyridyl)-biphenyl], and 4 [1,3-bis(4-pyridyl)-benzene] employed in this work. b Schematic illustration of the coordination motifs achieved in this work. The angles between the ligands approaching to the same Ce atom are marked by α.
2 NATURE COMMUNICATIONS | (2021) 12:1619 | https://doi.org/10.1038/s41467-021-21911-z | www.nature.com/naturecommunications NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-021-21911-z ARTICLE
a b c
0 Δz (Å)2.6 0 Δz (Å) 3.2 0 Δz (Å) 3.2
Fig. 2 Coordination structures involving Ce and 1 formed on Au(111). STM images of a the single-wall honeycomb structure (scanning conditions: bias V = −10 mV, tunneling current I = −30 pA, imaging temperature T = 77 K), b the Kagome structure (V = 5 mV, I = 50 pA, T = 77 K), and c the double- wall honeycomb structure (V = 30 mV, I = 100 pA, T = 77 K) formed by depositing 1 and Ce on Au(111). The structural motifs constructing the coordination structures are illustrated by the superimposed molecular models. Color code: dark gray for C, white for H, blue for N, light green for Ce, and orange for Au adatom. The unit cells are highlighted by the white parallelograms. Scale bars: 2 nm.
a b c
0 Δz (Å) 1.3 0 Δz (Å) 2.3 0 Δz (Å) 1.3
Fig. 3 Coordination structures involving Ce and 2 formed on Au(111). STM images of a a quasi-fourth-order Sierpinskí triangle (V = 100 mV, I = 20 pA, T = 77 K), b the three-lobe structure (V = 10 mV, I = 20 pA, T = 4.3 K), and c the four-lobe structure (V = 10 mV, I = 200 pA, T = 4.3 K) formed by ́ depositing 2 and Ce on Au(111). Inset of a: Magniﬁed image of the Ce(CN)3 building block of the Sierpinski triangles. The orientations of the Ce dimers in the three-lobe structure are marked by the green and blue arrows in b. The unit cells are highlighted by the white parallelograms in b and c. The structural motifs constructing the coordination structures are illustrated by the superimposed molecular models. Scale bars: a 5 nm, b 2 nm, and c 2 nm. the single-wall honeycomb structure. Accordingly, a model of the the double-wall honeycomb networks feature the multi-Ce- coordination network formed by Ce and 1 is proposed. In this containing clusters as the coordination centers. The clusters are model, three molecules 1 approach to a Ce atom with their organized through their coordination with the molecular ligands pyridine ends to form coordination bonds between the pyridine- into the ordered 2D arrays. The 2D networks can be described by N atoms and the Ce atom. This gives rise to the threefold the hexagonal unit cells as marked by the white parallelograms in mononuclear coordination node as the building block, denoted as Fig. 2b, c with dimensions of 3.4 and 3.1 nm, respectively. the CePy3 motif, as illustrated by the superimposed molecular models in Fig. 2a. Subsequent thermal treatment of the sample at about Coordination structures involving Ce and nitrile ligand 2 355–375 K resulted in the partial desorption of the molecular formed on Au(111). In order to enrich the diversity of the ligands, which led to a decreased molecule-to-Ce ratio involved in Ce-engaged coordination structures, we employed the nitrile the coordination structures as compared with that in the single- molecule 2 (Fig. 1a) instead of the pyridine molecule 1 as the wall honeycomb network, that is, 3:2. As a consequence, two new ligand to construct coordination structures with Ce on Au(111). structures with a lower molecule-to-Ce ratio (1:1) emerged, i.e., Without Ce adatoms, molecules 2 were found to assemble into the Kagome network (Fig. 2b and Supplementary Fig. 2a) and the the braid-like structures via intermolecular hydrogen bonds on double-wall honeycomb network (Fig. 2c and Supplementary Au(111) at room temperature (Supplementary Fig. 3). As a Fig. 2b). The STM image of the Kagome structure (Fig. 2b) clearly comparison, coordinated Sierpiński triangles11–13 (Fig. 3a and resolves two identical bright dots (highlighted by the light green Supplementary Fig. 4a) were obtained by depositing Ce onto the dots) at the center of each fourfold node (molecular models 2-precovered Au(111) substrate held at room temperature, indi- superimposed), which are assigned as two Ce atoms. As for the cating the engagement of Ce atoms in the fractal structures. The double-wall honeycomb network (Fig. 2c), one can see three building block of the Sierpiński triangles is the coordination motif bright dots in the STM image (marked by the light green dots) formed by one Ce atom approached by three nitrile molecules, ﬁ which are identi ed as a Ce trimer at the center of six molecular denoted as Ce(CN)3, as illustrated by the superimposed molecular ligands (molecular models superimposed). Both the Kagome and models in Fig. 3a inset.
NATURE COMMUNICATIONS | (2021) 12:1619 | https://doi.org/10.1038/s41467-021-21911-z | www.nature.com/naturecommunications 3 ARTICLE NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-021-21911-z
By depositing more Ce atoms to the sample with the hexagonal unit cell of 2.2 nm (Fig. 4b and Supplementary Fig. 6c). coordinated Sierpiński triangles on the Au(111) substrate The engagement of 4 leads to a chain-like structure with a 1D followed by thermal treatment of the sample at about 350 K, a periodicity of 1.3 nm (Fig. 4c and Supplementary Fig. 7b). Besides three-lobe structure and a four-lobe structure were obtained these Ce-dimer-based structures, a low yield of the coordination (Fig. 3b, c and Supplementary Fig. 4b). Figure 3b shows the motifs formed by the three-Ce-containing clusters and ligand 3 representative STM image of the three-lobe structure, in which was also observed (Supplementary Fig. 6d). the two bright dots (highlighted by the light green dots) located at Next, the coordination of Ce with either 1 or 2 was investigated on the center of six molecules (molecular models superimposed) are Au(100). As a result, the ﬁshing-net structure (Supplementary assigned as two Ce atoms. The orientation of the Ce dimers, as Fig. 8a, b) and the double-wall honeycomb network (Supplementary marked by the green and blue arrows in Fig. 3b, varies regularly Fig. 8a, c) formed by the pyridine ligand 1 and the two- or three-Ce- within the domain (Supplementary Fig. 5). The unit cell of the containing clusters, as well as the three-lobe (Supplementary Fig. 8d, e) three-lobe network is highlighted by the white parallelogram in and four-lobe (Supplementary Fig. 8d, f) structures formed by the Fig. 3b with the dimensions of a = 3.4 nm, b = 6.8 nm, and an nitrile ligand 2 and the two- or four-Ce-containing clusters were all angle of about 60o between them. Coexisting with the three-lobe obtained on Au(100). network, the four-lobe coordination structure (Fig. 3c) features a square unit cell as marked by the white frame in Fig. 3c with a periodicity of 2.3 nm. Four bright dots are discernible in the high- Structures of the coordinated multi-Ce-containing clusters. resolution STM image (marked by the light green dots in Fig. 3c) The experimental observation of the coordinated clusters com- which are assigned as four Ce atoms at the center of eight prising 2, 3, and 4 Ce atoms distinguishes the Ln-engaged on- molecules (molecular models superimposed in Fig. 3c). surface coordination system studied in this work from most of the previously reported ones in which single Ln atoms were identiﬁed as the coordination centers14–24. To elucidate the structure of the Coordination of Ce with different molecules and on different multi-Ce-containing clusters, as well as to ﬁgure out the intra- substrates. To extend the range of conditions applicable for the cluster and cluster–ligand interactions, combined experimental on-surface preparation of the multi-Ce-containing clusters, as and theoretical studies were carried out. The results reveal the well as to achieve various assemblies of the clusters, the coordi- heterometallic nature of the clusters, showing that the Ce atoms nation of Ce with different molecules and on varied lattice planes in the clusters are stabilized by the bridging Au adatoms, as of Au substrate were studied. demonstrated below. Firstly, we employed molecules 3 and 4 (Fig. 1a) as the ligands First of all, the Ce–Au binary surface system in the absence of to construct coordination structures with Ce on Au(111). Both molecular ligands is considered. It is documented that the molecules possess pyridine coordination groups but show preparation of 2D LnAu2 intermetallic compounds has been different backbone structures compared with the pyridine ligand achieved for a number of Ln metals, namely, La32,Ce32,33, 1. In addition to the mononuclear coordination structures Gd34–36,Tb37,38,Ho37, and Er37, by the surface alloying of Ln ﬁ constructed by the CePy3 motifs, i.e., the single-wall honeycomb with the Au(111) substrate. All these LnAu2 lms share the same network formed by Ce and 3 (Supplementary Fig. 6a) and the lattice structure in which each pair of the nearest-neighboring Ln coordinated Sierpiński triangles formed by Ce and 4 (Supple- atoms are bridged by two Au atoms32,34,35,37. Charge transfer mentary Fig. 7a), the multinuclear coordiantion structures were from Ln to Au was found in these systems34, which is in also achieved. Figure 4 shows the three-ordered structures accordance with the remarkable electronegativity difference assembled by the coordination between the Ce dimers and ligand between Ln and Au: Ln metals are highly electropositive while 3 or 4. The coordination of 3 with the two-Ce-containing clusters Au is the most electronegative metal on the Pauling scale39. The gives rise to a Kagome network (Fig. 4a and Supplementary electronegativity distinction and the charge transfer are supposed Fig. 6b) that shows a larger periodicity (4.5 nm) compared with to facilitate the Ln–Au intermixing but suppress the direct Ln–Ln that formed by 1 (Fig. 2b), and a ﬁshing-net structure with a bonding in the binary systems. Similar to Ln elements, other acb
8 I (pA) 384 0 Δz (Å)3.2 0 Δz (Å) 2.1
Fig. 4 Coordination structures involving Ce and 3 or 4 formed on Au(111). STM images of a the Kagome structure (in constant-height mode, V = 5 mV, I = 350 pA at the point marked by the cross, T = 77 K) and b the ﬁshing-net structure (V = 100 mV, I = 20 pA, T = 77 K) formed by depositing 3 and Ce on Au(111), and c the chain-like structure (V = −1 mV, I = −50 pA, T = 4.3 K) formed by depositing 4 and Ce on Au(111). The unit cells of the Kagome and the ﬁshing-net structures are highlighted by the white parallelograms in a and b. The 1D periodicity of the chain-like structure is marked by the white arrow in c. The structural motifs constructing the coordination structures are illustrated by the superimposed molecular models. Scale bars: a 2 nm, b 2 nm, and c 1 nm.
4 NATURE COMMUNICATIONS | (2021) 12:1619 | https://doi.org/10.1038/s41467-021-21911-z | www.nature.com/naturecommunications NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-021-21911-z ARTICLE electropositive metals, e.g., the alkali metals Na40,41,K42, and spectra exhibit two broad peaks (binding energies at ~885 and Cs43,44, have also been reported to form surface alloys with the 904 eV) that show negligible shifts with the varied molecule-to-Ce Au substrates. Therefore, it can be summarized from the ratios and different annealing temperatures of the samples literature that the atoms of the electropositive metals, such as (Supplementary Fig. 10b). The two peaks are characteristic of Ce Ce, usually intermix with Au atoms rather than directly bond alloying with Au, as demonstrated by the XPS studies of the Ce–Au with each other in the binary surface systems. surface alloy grown on Au(111) in this work (bottom curve in Next, we take the molecular ligands into account to Supplementary Fig. 10b) and the previous reports33,45. The fact demonstrate that the Ce atoms coordinated with the molecules that the positions of the Ce 3d peaks are independent from the are bridged by Au adatoms to form the multinuclear clusters preparation conditions of the samples suggests the similar chemical observed in this work. The experimental evidence comes from states of the Ce atoms in the coordination structures that comprise both the STM and X-ray photoelectron spectroscopy (XPS) metallic centers with different nuclearities. This is in agreement results. We conducted STM characterization of the large with the theoretical ﬁndings showing the similar charges carried by coordinated clusters with high nuclearities prepared by depositing the Ce atoms in the different coordination centers (about +2|e|per Ce and ligand 3 on Au(111) followed by 530 K annealing, aiming Ce atom), as described in detail below. It can be concluded from at comparing the large clusters with the Ce–Au surface the XPS results that the coordinated clusters are composed of intermetallic compound. As shown in Supplementary Fig. 9, intermixed Ce and Au atoms. clusters comprising seven or more bright dots that are assigned as The existence of bridging Au adatoms in the coordinated clusters Ce atoms are connected by the molecular ligands to construct the is also supported by the calculation results. We start from the less ordered coordination structure. Both Ce atoms that are building block of the three-lobe structure (Fig. 3b), i.e., the coordinated with the molecules (denoted as CeL, examples are coordination motif consisting of a Ce dimer and six nitrile ligands ﬁ marked by the blue dots in Supplementary Fig. 9) and those that 2, to interpret the theoretical ndings. Firstly, a Ce2(CN)6 model of are surrounded by the other Ce atoms (denoted as CeCe, examples the coordination motif in which the coordination center is formed are marked by the red dots in Supplementary Fig. 9) can be found by two directly approached Ce atoms was theoretically tested. The – ﬁ in the multinuclear clusters. Measurement of the CeL CeL, optimized structure of Ce2(CN)6 in which the simpli ed nitrile – – CeCe CeL, and CeCe CeCe distances leads to the similar results of ligands were employed is displayed in Supplementary Fig. 11a. 5.0 ± 0.5, 5.1 ± 0.4, and 5.0 ± 0.5 Å, respectively. All these values The calculation reveals a positive charge of +1.98 |e| for each Ce – ﬁ are comparable to the Ce Ce separation in the CeAu2 lm grown atom due to the charge transfer between the Ce atoms and the Au on Au(111), that is, 5.4 Å32. Moreover, the arrangement of the Ce substrate. The approaching of the two positively charged Ce atoms atoms in the clusters, although distorted more or less due to the thus leads to a repulsive interaction between them, which is asymmetric interactions of the molecular ligands, roughly responsible for the positive (i.e., unstable) Ce–Cebindingenergyof ﬁ resembles the hexagonal lattice of the Ce atoms in the CeAu2 0.30 eV, and the electron de ciency between the two Ce atoms as intermetallic compound prepared on Au(111)32,33. These results seen in the differential electron density map (Supplementary suggest that, on the one hand, the CeCe atoms are highly likely to Fig. 11b). These results exhibit the reduced stability of the structure be connected with each other in the same way as that in the caused by the direct approaching of the two Ce atoms. Moreover, CeAu2 surface alloy, i.e., to be bridged by Au adatoms, and on the one can see the slight lift-up of the substrate Au atom between the other hand, the bridging Au adatoms are also responsible for the two Ce atoms (Supplementary Fig. 11a), which is supposed to – – – CeCe CeL and CeL CeL connections given the similar Ce Ce suppress the lateral movement of the coordinated Ce dimer since separations and arrangements of the CeCe and CeL atoms in the such a process requires frequent reconstruction of the substrate. large clusters. The analyses provide clues for identifying the two-, However, in contrast to the calculation results, the tip-manipulation three-, and four-CeL-containing clusters in the ordered coordina- experiment shows the lateral displacements of the coordination tion structures as the Ce–Au heterometallic clusters. motif formed by a Ce dimer and six nitrile ligands as a whole (see Furthermore, in order to ﬁgure out the chemical state of the Ce Supplementary Fig. 12 and Supplementary Discussion for details), atoms in the coordinated clusters, XPS measurements were carried and hence rejects the Ce2(CN)6 model. out for the samples with Ce and ligand 2 on Au(111). Different Subsequently, two models with one or two bridging Au adatom molecule-to-Ce ratios and annealing temperatures were employed (s) located between the two Ce atoms, i.e., Ce2Au(CN)6 and for preparing the samples to reproduce the different coordination Ce2Au2(CN)6, respectively, were tested. The atomic arrangement structures. We found shift of C 1s signal toward higher binding of the Ce2Au2 cluster in the latter model is proposed according to energy by increasing the coverage of Ce (Supplementary Fig. 10a), the lattice structure of the CeAu2 surface intermetallic compound which is attributed to the charge transfer from the ligands to the Ce grown on Au(111)32. The optimized models of the two candidate atoms caused by the coordination between them. The Ce 3d structures are displayed in Supplementary Fig. 13a and Fig. 5a,
acb +0.005 e/Bohr 3 -0.005
Fig. 5 Theoretical results of the Ce2Au2(CN)6 structure. a DFT optimized models (upper: top view, lower: side view), b simulated STM image, and c cross-section of the differential electron density along the black dashed line in a of the Ce2Au2(CN)6 motif on Au(111). Simpliﬁed molecular ligands are employed.
NATURE COMMUNICATIONS | (2021) 12:1619 | https://doi.org/10.1038/s41467-021-21911-z | www.nature.com/naturecommunications 5 ARTICLE NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-021-21911-z respectively. The calculations reveal that the energy of the charges on the Au adatoms (−0.47 |e| per Au adatom, Table 1). + Ce2Au2(CN)6 [Ce2Au(CN)6] structure is 1.57 eV (0.75 eV) lower The whole coordination motif is positively charged ( 3.21 |e|) (i.e., more stable) than the total energy of the Ce2(CN)6 motif plus and is stabilized by the substrate. These results demonstrate a two (one) non-interacting Au adatom(s). Note that the Au remarkable charge transfer from the Ce atoms to the Au adatoms adatom absorbed on the terrace of the substrate is taken as the and the Au substrate, which is similar to the situation in the reference state for the energy calculation here, whereas the Au Ce–Au binary systems as mentioned above. Therefore, the adatoms on the Au substrate are usually stabilized by re-attaching bridging Au adatoms play an indispensable role in the formation to the step edges in the real conditions. In the latter context, the of the two-Ce-containing clusters by serving as the negatively energy differences between the proposed structures with and charged “glue” to hold the two positively charged Ce atoms without the bridging Au adatom(s) can be estimated by together. subtracting the formation energy of the adatom(s) emitted from The crucial role of the Au adatoms in stabilizing the 46 ﬁ the step (0.500 eV per Au adatom ) from the above-presented Ce2Au2(CN)6 motif is further con rmed by the formation of results. This gives rise to the energy differences of 0.57 and direct Ce–Au bonds in the Ce2Au2 cluster as demonstrated by our – 0.25 eV for Ce2Au2(CN)6 and Ce2Au(CN)6, respectively, lower theoretical investigations as follows. The averaged Ce Au distance than Ce2(CN)6, which still indicates an energetic preference for (dCe–Au) in the optimized Ce2Au2(CN)6 model (Fig. 5a) is 3.02 Å formation of the structures with the bridging Au adatom(s). (Table 2), which is smaller than the sum of their covalent radii Given that Au adatoms generated from the step and diffusing on (3.14 Å)39, implying the formation of unsupported Ce–Au bonds. – tot the terrace should be well accessible on Au(111) under the The calculation of the total Ce Au binding energy (ECeÀAu) in the 46–50 reaction conditions , we propose the most energetically Ce2Au2(CN)6 motif reveals an appreciable energy gain achieved by preferred Ce2Au2(CN)6 structure among the proposed models forming four direct Ce–Au bonds in the multinuclear cluster, that as the building block of the three-lobe structure, as illustrated by is, 3.03 eV in value (Table 2, also see “Methods” for details of the superimposed molecular models in Fig. 3b. The similar the binding energy calculation). This exhibits the key effect of the phenomenon was also found by Yan et al.30 showing that the Ce–Au interactions in stabilizing the coordination structure. The evaporated metal atoms were bridged by the intrinsic adatoms to formation of Ce–Au bond is further supported by the differential – form coordinated heterometallic clusters on surfaces. The Ce Ce electron density map of the Ce2Au2(CN)6 structure (Fig. 5c). distance in the optimized model of the Ce2Au2(CN)6 motif The cross-section of the differential electron density depicts the (4.95 Å) is consistent with the experimental value (4.7 ± 0.4 Å) by electron accumulation (red) and deﬁciency (blue) due to the taking the measurement error into account. Moreover, the formation of the coordination motif (see “Methods” for details of simulated STM image of the optimized Ce2Au2(CN)6 structure the calculation of differential electron density). It is clearly seen in (Fig. 5b) was compared with those of Ce2(CN)6 (Supplementary Fig. 5c that electron density intensiﬁes between the Ce and Au Fig. 11c) and Ce2Au(CN)6 (Supplementary Fig. 13b). As a result, atoms, indicative of the direct Ce–Au bond formation. the STM simulation of Ce2Au2(CN)6 shows the best agreement As for the cluster–ligand interaction, the optimized model of ﬁ with the experimental data, which supports the identi cation of the Ce2Au2(CN)6 motif (Fig. 5a) shows the coordination of three the Ce2Au2(CN)6 structure as the coordination motif to construct nitrile molecules to each Ce atom in the Ce2Au2 cluster. the three-lobe network. In both experimental images and STM The averaged Ce–N distance is 2.53 Å (Table 2), which falls in 14,16,22 simulation of Ce2Au2(CN)6, the two Ce atoms are resolved as the the range of nitrile–Ce coordination bond length . The – − two bright dots while the Au adatoms are invisible. This can be averaged binding energy for each Ce N bond (ECeÀN)is 1.30 eV understood by the larger atomic radius of Ce than Au which leads (Table 2, also see “Methods” for details of the binding energy to a larger height in z direction of the former than the latter when calculation). they are adsorbed on the Au substrate, as displayed by the side Given the critical role of the bridging Au adatoms in stabilizing view of the optimized model (Fig. 5a bottom). The similar the Ce2Au2(CN)6 structure, we argue that the coordination centers situation that only the metal atoms with a bigger size in the of all the other multinuclear coordination structures achieved in heterometallic clusters are discernable by STM was also reported this work are composed of the Ce–Au heterometallic clusters in by Yan et al. recently30. which each pair of the nearest-neighboring Ce atoms are bridged The higher stability of Ce2Au2(CN)6 than Ce2(CN)6 suggests by two Au adatoms, as proposed according to the atomic 32 that the existence of the bridging Au adatoms in the arrangement of the CeAu2 surface alloy prepared on Au(111) Ce2Au2(CN)6 motif facilitates the stabilization of the coordinated (see Supplementary Fig. 14 and Supplementary Discussion for cluster. In order to get insights into the stabilization effect of the other tested models of the coordinated four-Ce-containing bridging Au adatoms, Bader charge analysis of the Ce2Au2(CN)6 cluster). The optimized models are presented in Fig. 6a–c, showing motif was carried out. The calculations uncover positive charges the Ce2Au2Py4 motif as the building block of the Kagome (Figs. 2b on the Ce atoms (+1.98 |e| per Ce atom, Table 1) and negative and 4a), ﬁshing-net (Fig. 4b), and chain-like (Fig. 4c) structures, while the double-wall honeycomb (Fig. 2c) and four-lobe (Fig. 3c) structures are constructed by the Ce Au Py and Ce Au (CN) – 3 4 6 4 5 8 Table 1 Bader charges of the Ce Au clusters in the motifs, respectively, as illustrated by the molecular models coordination motifs. superimposed in Figs. 2b, c, 3c, and 4.TheCe–Ce distances in these models, i.e., 4.52 Å for Ce2Au2Py4, 5.56 Å for Ce3Au4Py6, e Motif Charge (| |) and 4.77 Å for Ce4Au5(CN)8, are consistent with the experimen- tally measured values, that is, 4.5 ± 0.3, 5.1 ± 0.5, and 4.9 ± 0.5 Å, Ce Au respectively. Note that the orientations of the coordination motifs + − Ce2Au2Py4 1.88 0.59 – + − with respect to the substrate as shown in Figs. 5a and 6a c have all Ce3Au4Py6 1.85 0.49 (for peripheral Au) been conﬁrmed by the experimental observations. Bader charges −0.56 (for central Au) of the Ce and Au atoms in these multinuclear motifs are listed in Ce2Au2(CN)6 +1.98 −0.47 + − Table 1, exhibiting that the positively charged Ce atoms are Ce4Au5(CN)8 1.87 0.51 (for peripheral Au) – −0.76 (for central Au) bridged by the negatively charged Au adatoms. The direct Ce Au interactions in these structures are supported by the dCe–Au values
6 NATURE COMMUNICATIONS | (2021) 12:1619 | https://doi.org/10.1038/s41467-021-21911-z | www.nature.com/naturecommunications NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-021-21911-z ARTICLE
Table 2 Lengths and Energies of the Ce–Au and Ce–N bonds in the coordination motifs.
tot Motif dCe–Au (Å) ECeÀAu (eV) dCe–N (Å) ECe–N (eV)
Ce2Au2Py4 2.98 −3.38 2.59 −1.33 Ce3Au4Py6 3.04 (for Ce-peripheral Au) 3.21 (for Ce-central Au) −5.41 2.61 −1.31 Ce2Au2(CN)6 3.02 −3.03 2.53 −1.30 Ce4Au5(CN)8 2.93 (for Ce-peripheral Au) 3.39 (for Ce-central Au) −8.69 2.55 −1.17
Ce2Au2Py4 Ce3Au4Py6 Ce4Au5(CN)8 a bc
-0.005 e/Bohr3 +0.005
Fig. 6 Theoretical results of the multinuclear coordination structures. Optimized models of a the Ce2Au2Py4, b the Ce3Au4Py6, and c the Ce4Au5(CN)8 motifs (upper: top view, lower: side view). Cross-sections of the differential electron densities of d the Ce2Au2Py4, e the Ce3Au4Py6, and f the Ce4Au5(CN)8 motifs along the black dashed lines in a, b and c, respectively.
(Table 2) that are comparable with the sum of covalent radii of Ce Ce2Au2(CN)6 and Ce4Au5(CN)8. It is found that the nitrile- and Au (3.14 Å)39, as well as the large total Ce–Au binding engaged multinuclear motifs show smaller angles between the tot “ ” α energies (ECeÀAu in Table 2,see Methods for details of the ligands approaching to the same Ce atom [marked by in Fig. 1b; α – o binding energy calculations). The differential electron density ~60 70 for Ce2Au2(CN)6 and Ce4Au5(CN)8] than the ones maps of the three multinuclear motifs (Fig. 6d–f) provide another formed by the pyridine ligands (α ~ 120o). This can be explained evidence for the unsupported Ce–Au bonds by presenting the by the smaller volume of the nitrile group than the pyridine electron density accumulation between the Ce and Au atoms in group, which allows for the approaching of the nitrile ligands to these structures. As for the cluster–ligand interactions in the three the same metal atom with a relatively small coordination angle multinuclear motifs, it is seen in the optimized models (Fig. 6a–c) without introducing signiﬁcant steric hinderance. The different that the coordination interactions are formed between the coordination behaviors of the pyridine and nitrile ligands with the molecular ligands and the Ce atoms in the Ce–Au clusters. The Ce–Au clusters give rise to the various ordered coordination calculated Ce–ligand distances and binding energies are summar- assemblies observed in this work, showing the feasibility of uti- ized in Table 2. lizing different molecular ligands to tune the organization and periodicity of the Ce–Au cluster arrays. Next, we discuss the possible mechanism for the formation of Discussion the multinuclear coordination structures. All the multinuclear Firstly, we compared the multinuclear coordination motifs coordination structures achieved in this work feature relatively formed by the pyridine ligands 1, 3, and 4, i.e., Ce2Au2Py4 and low molecule-to-Ln ratios (no more than 3:2). Each Ce atom in Ce3Au4Py6, with those constructed by the nitrile ligand 2, i.e., these structures coordinates with two or three molecular ligands.
NATURE COMMUNICATIONS | (2021) 12:1619 | https://doi.org/10.1038/s41467-021-21911-z | www.nature.com/naturecommunications 7 ARTICLE NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-021-21911-z
As a comparison, relatively high molecule-to-Ln (or molecular nitrile (2) ligands on the Au(111) and Au(100) substrates, coordination site-to-Ln in the case of chelating ligands being yielding orderly arranged mono-dispersed Ce–Au cluster arrays. engaged) ratios (3:2 or higher) were frequently found for the The Au adatoms serve as the atomic “glue” to bridge the Ce previously reported Ln-engaged mononuclear coordination atoms via the unsupported Ce–Au bonds, as demonstrated by the structures constructed on surfaces14–24, in which the single Ln DFT calculations, which play a crucial role in stabilizing the atoms afforded multi (≥3)-fold coordination with the molecular heterometallic clusters. These results shed light on the application ligands. Accordingly, we propose that the low molecule-to-Ln of on-surface coordination as an efﬁcient strategy for the pre- ratios employed for the preparation of the metal-organic hybrids paration and organization of TM-bridged heterometallic clusters in this work should play a key role in the formation of the containing multiple Ln atoms which are of great signiﬁcance at multinuclear coordination structures. both fundamental and applied levels. One may expect two types of coordination products in the samples with a molecule-to-Ln ratio ≤3:2, i.e., the mononuclear Methods structures with low coordination numbers (namely, two- or Sample preparation, STM, and XPS measurements. The samples were prepared threefold coordination), and the multinuclear structures. The in UHV preparation chambers connected with either the STM or XPS chamber. Au (111) and Au(100) surfaces were cleaned by repeated cycles of Ar+ sputtering and comparison of the stability of these two types of coordination annealing. Molecules 1, 2, 3, and 4 were thermally sublimated from the tantalum structures can be carried out based on the calculation results boats. Ce was evaporated from an electron-beam evaporator at about 1420 K. The shown above. For the two- and threefold mononuclear struc- thermal treatment of the samples was carried out with a temperature control within tures, the stabilizing energy per Ce atom due to the formation of ±20 K. All STM experiments were carried out with a Unisoku UHV-STM with a base pressure lower than 3 × 10−10 Torr in the system. STM images were acquired the coordination bonds with the ligands can be estimated as ﬁ − − in constant-current mode if not otherwise speci cally stated and were processed by about 2.6 and 3.9 eV, respectively, by taking the averaged the WSxM software55. All XPS experiments were carried out in a SPECS system Ce–N binding energy of the coordination structures concerned with a monochromatic Al Kα X-ray source (hν = 1486.6 eV). The base pressure of −10 in this work for evaluation. As for the multinuclear structures the system is lower than 5 × 10 Torr. The Au 4f7/2 peak of a clean Au(111) constructed by the Ce Au Py ,CeAu Py ,CeAu (CN) ,or substrate was used to calibrate the spectrometer before experiments. The Au 4f5/2 2 2 4 3 4 6 2 2 6 peak of the Au(111) substrate at 87.7 eV was employed as an internal standard to Ce4Au5(CN)8 motifs, the stabilizing energy per Ce atom con- calibrate the binding energy scale for this work. tributed by the bonding with both the molecular ligands and the − − Au adatoms ranges from 4.4 to 5.4 eV. As a conclusion, the Calculation methods. All DFT calculations were performed using the projected multinuclear coordination structures are thermodynamically augmented-wave (PAW) pseudopotentials56,57, as implemented in Vienna Ab preferred at low molecule-to-Ln ratios. Thus, the reduction in initio Simulation Package (VASP)58. The exchange-correlation energy was calcu- the molecule-to-Ln ratio of the sample, which can be achieved lated with the opt-B88 functional in order to take the van der Waals (vdW) dispersive correction into consideration59–61. Scalar relativistic effect which by either deposition of additional Ce or molecular desorption includes the mass-velocity and Darwin correction terms, as implemented in caused by thermal treatment of the sample, can serve as a VASP62, was taken into account. The potential of Ce was generated with 12 valence driving force for the emergence of the multinuclear coordination electrons including the 4f electron. The cut-off energy was 400 eV for the structures. Kohn–Sham wave functions. A vacuum space of 10 Å was applied between neighboring structures to ensure their decoupling. The initial geometries of the Moreover, thermal treatment of the sample is also necessary for Ce–Au clusters in the models for optimization were set either according to the 32 the preparation of the multinuclear structures. In addition to lattice structure of the CeAu2 intermetallic compound prepared on Au(111) ,or tuning the molecule-to-Ln ratio by the thermal-induced mole- by referring to the parameters achieved in other optimized structures studied in cular desorption as mentioned above, the thermal treatment also this work. The geometry was fully optimized when the maximum forces fell down below 0.02 eV Å−1.AΓ centered grid was applied for the Brillouin zone sampling. provides energies for the diffusion and rearrangement of the – tot The total Ce Au binding energy (ECeÀAu) of the CemAunLk (L for ligand) motif molecules and metal adatoms on the surface, which is indis- is calculated as below pensable for obtaining the thermodynamically preferred multi- tot E À ¼ E = À E = À E = þ E ð1Þ nuclear products. Otherwise, coordination structures with lower Ce Au CemAun Lk sub CemLk sub Aun sub sub in which E = , E = , E = , and E refer to the energies of the stability may emerge, such as the threefold mononuclear struc- CemAun Lk sub CemLk sub Aun sub sub tures (namely, the single-wall honeycomb network formed by 1 CemAunLk motif on the substrate, the CemLk fragment on the substrate, the Au ́ 2 adatoms on the substrate, and the Au(111) substrate, respectively. Here, the Au and the Sierpinski triangles formed by ) obtained at room adatom on the terrace of the substrate is taken as the reference state for the energy temperature in this work. calculation. The total Ce–Au binding energy relative to the Au atom at the step Last but not least, we have taken the three- and four-lobe edge can be estimated by adding the formation energy of the Au adatoms emitted 46 tot structures constructed by the Ce Au (CN) and Ce Au (CN) from the step on Au(111) (0.500 eV per atom )toECeÀAu. The so-achieved results 2 2 6 4 5 8 – motifs, respectively, as examples to explore the magnetic and still represent considerable stabilization effect of the Ce Au bonds. The Ce–N binding energy (E – ) of the Ce Au L motif is calculated as below electronic properties of the Ce–Au clusters by STS experiments. Ce N m n k – E À ¼ðE = À E = À E = þ E Þ=k ð2Þ However, we failed to get any magnetic signals of the Ce Au Ce N Cem Aun Lk sub CemAun sub Lk sub sub clusters by high-resolution dI/dV measurement. The similar in which E = and E = refer to the energies of the Ce Au cluster on the CemAun sub Lk sub m n situations have been reported for some surface-conﬁned double- substrate and the molecular ligands on the substrate, respectively. decker lanthanide phthalocyanine molecules whose 4f electron The differential electron density (dρ) is calculated as below – 51 54 ρ ¼ ρ À ρ À ρ À ρ À ρ ð Þ states were elusive to be detected by STS measurement . The d tot Ce Au L sub 3 reason may lie in the inner-core nature of the 4f orbitals which ρ ρ ρ ρ ρ where tot, Ce, Au, L, and sub correspond to the electron densities of the total leads to the little contribution of the 4f electron of Ce to the system, the Ce atom, the Au adatom, the molecular ligand, and the substrate, tunneling current. We neither found any Ce-speciﬁcdI/dV fea- respectively. ture in the large range (−4 to 3 V) dI/dV spectra. It may be explained by the strong hybridization between the Au substrate Data availability and the Ce–Au clusters. The data that support the ﬁndings of this study are available within the paper and its To summarize, a series of heterometallic clusters containing 2, supplementary information ﬁle. Raw data are available from the corresponding author 3, and 4 Ce atoms bridged by Au adatoms were prepared with an upon reasonable request. on-surface coordination strategy in UHV. STM investigations reveal the formation of ordered coordination structures based on Received: 21 August 2020; Accepted: 19 February 2021; the well-deﬁned Ce–Au clusters and the pyridine (1, 3 and 4)or
8 NATURE COMMUNICATIONS | (2021) 12:1619 | https://doi.org/10.1038/s41467-021-21911-z | www.nature.com/naturecommunications NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-021-21911-z ARTICLE
References 31. Zhang, X. et al. Inﬂuence of relativistic effects on assembled structures of 1. Fidler, J., Suess, D. & Schreﬂ,T.Handbook of Magnetism and Advanced V-shaped bispyridine molecules on M(111) surfaces where M = Cu, Ag, Au. Magnetic Materials Vol. 4 (Wiley, 2007). ACS Nano 11, 8511–8518 (2017). 2. David, E. An overview of advanced materials for hydrogen storage. J. Mater. 32. Ormaza, M. et al. LaAu2 and CeAu2 surface intermetallic compounds grown Process Technol. 162–163, 169–177 (2005). by high-temperature deposition on Au(111). Phys. Rev. B 88, 125405 (2013). 3. Huang, Y.-G., Jiang, F.-L. & Hong, M.-C. Magnetic lanthanide-transition- 33. Ma, S., Zhao, X., Rodriguez, J. A., Hrbek, J. & STM, X. P. S. study of growth of metal organic-inorganic hybrid materials: from discrete clusters to extended Ce on Au(111). J. Phys. Chem. C 111, 3685–3691 (2007). – frameworks. Coord. Chem. Rev. 253, 2814 2834 (2009). 34. Corso, M. et al. Rare-earth surface alloying: a new phase for GdAu2. Phys. Rev. 4. Liddle, S. T. & Mills, D. P. Metal-metal bonds in f-element chemistry. Dalton Lett. 105, 016101 (2010). Trans. https://doi.org/10.1039/b904318g (2009). 35. Corso, M., Fernández, L., Schiller, F. & Ortega, J. E. Au(111)-based 5. Butovskii, M. V. et al. Molecules containing rare-earth atoms solely bonded by nanotemplates by Gd alloying. ACS Nano 4, 1603–1611 (2010). transition metals. Nat. Chem. 2, 741–744 (2010). 36. Fernández, L. et al. Self-organized growth of high density magnetic Co 6. Oelkers, B., Butovskii, M. V. & Kempe, R. f-Element-metal bonding and the nanodot arrays on a Moiré template. Appl. Phys. Lett. 96, 013107 (2010). use of the bond polarity to build molecular intermetalloids. Chem. Eur. J. 18, 37. Que, Y. et al. Two-dimensional rare earth-gold intermetallic compounds on 13566–13579 (2012). Au(111) by surface alloying. J. Phys. Chem. Lett. 11, 4107–4112 (2020). 7. Butovskii, M. V. et al. Lanthanoid-transition-metal bonding in 38. Que, Y. et al. On-surface synthesis of graphene nanoribbons on two- bismetallocenes. Chem. Eur. J. 20, 2804–2811 (2014). dimensional rare earth-gold intermetallic compounds. J. Phys. Chem. Lett. 11, 8. Butovskii, M. V., Tok, O. L., Bezugly, V., Wagner, F. R. & Kempe, R. 5044–5050 (2020). Molecular lanthanoid-transition-metal cluster through C-H bond activation 39. Haynes, W. M. (ed.). CRC Handbook of Chemistry and Physics 95th edn (CRC by polar metal-metal bonds. Angew. Chem. Int. Ed. 50, 7695–7698 (2011). Press, 2014). 9. Dong, L., Gao, Z. A. & Lin, N. Self-assembly of metal-organic coordination 40. Barth, J. V., Brune, H., Schuster, R. & Ertl, G. Intermixing and two- structures on surfaces. Prog. Surf. Sci. 91, 101–135 (2016). dimensional alloy formation in the Na/Au(111) system. Surf. Sci. Lett. 292, 10. Lin, T., Kuang, G., Wang, W. & Lin, N. Two-dimensional lattice of out-of- L769–L774 (1993). plane dinuclear iron centers exhibiting kondo resonance. ACS Nano 8, 41. Barth, J. V., Behm, R. J. & Ertl, G. Adsorption, surface restructuring and alloy 8310–8316 (2014). formation in the Na/Au(111) system. Surf. Sci. 341,62–91 (1995). 11. Zhang, X. et al. Controlling molecular growth between fractals and crystals on 42. Barth, J. V., Schuster, R., Behm, R. J. & Ertl, G. The system K/Au(111): surfaces. ACS Nano 9, 11909–11915 (2015). adsorption and surface restructuring. Surf. Sci. 348, 280–286 (1996). 12. Li, C. et al. Construction of Sierpiński triangles up to the ﬁfth order. J. Am. 43. Wertheim, G. K., Rowe, J. E., Chiang, C.-M., Malic, R. A. & Buchanan, D. N. Chem. Soc. 139, 13749–13753 (2017). E. Surface properties of the semiconductor CsAu. Surf. Sci. 330,27–33 (1995). 13. Zhang, X. et al. One-dimensional molecular chains formed by Sierpiński 44. Knat’ko, M. V., Lapushkin, M. N. & Paleev, V. I. Initial stages in the formation triangles on Au(111). RSC Adv. 8, 1852–1856 (2018). of a CsAu surface alloy. Tech. Phys. Lett. 24, 390–392 (1998). 14. Écijaa, D. et al. Five-vertex archimedean surface tessellation by lanthanide- 45. Zhao, X., Ma, S., Hrbek, J. & Rodriguez, J. A. Reaction of water with Ce-Au directed molecular self-assembly. Proc. Natl Acad. Sci. USA 110, 6678–6681 (111) and CeOx/Au(111) surfaces: photoemission and STM studies. Surf. Sci. (2013). 601, 2445–2452 (2007). 15. Bischoff, F. et al. Metalation of porphyrins by lanthanide atoms at interfaces: 46. Stoltze, P. Simulation of surface defects. J. Phys. Condens. Matter 6, 9495–9517 direct observation and stimulation of cerium coordination to 2H-TPP/Ag (1994). (111). J. Phys. Chem. C 122, 5083–5092 (2018). 47. Sun, Q., Cai, L., Ma, H., Yuan, C. & Xu, W. Dehalogenative homocoupling of 16. Ecija, D., Urgel, J. I., Seitsonen, A. P., Auwarter, W. & Barth, J. V. Lanthanide- terminal alkynyl bromides on Au(111): incorporation of acetylenic scaffolding – directed assembly of interfacial coordination architectures-from complex into surface nanostructures. ACS Nano 10, 7023 7030 (2016). networks to functional nanosystems. Acc. Chem. Res. 51, 365–375 (2018). 48. Rastgoo-Lahrood, A. et al. From Au-thiolate chains to thioether Sierpinski 17. Cirera, B. et al. Dysprosium-carboxylate nanomeshes with tunable cavity size triangles: the versatile surface chemistry of 1,3,5-tris(4-mercaptophenyl) – and assembly motif through ionic interactions. Chem. Commun. 52, benzene on Au(111). ACS Nano 10, 10901 10911 (2016). 11227–11230 (2016). 49. Zhang, H. & Chi, L. Gold-organic hybrids: on-surface synthesis and – 18. Cirera, B. et al. Long-range orientational self-assembly, spatially controlled perspectives. Adv. Mater. 28, 10492 10498 (2016). deprotonation, and off-centered metalation of an expanded porphyrin. J. Am. 50. Liu, M. et al. Graphene-like nanoribbons periodically embedded with four- Chem. Soc. 139, 14129–14136 (2017). and eight-membered rings. Nat. Commun. 8, 14924 (2017). 19. Lyu, G. et al. Tunable lanthanide-directed metallosupramolecular networks by 51. Komeda, T. et al. Observation and electric current control of a local spin in a exploiting coordinative ﬂexibility through ligand stoichiometry. Chem. single-molecule magnet. Nat. Commun. 2, 217 (2011). Commun. 52, 1618–1621 (2016). 52. Schwöbel, J. et al. Real-space observation of spin-split molecular orbitals of 20. Urgel, J. I. et al. Quasicrystallinity expressed in two-dimensional coordination adsorbed single-molecule magnets. Nat. Commun. 3, 953 (2012). networks. Nat. Chem. 8, 657–662 (2016). 53. Yajie, Z. et al. Low-temperature scanning tunneling microscopy study on the 21. Urgel, J. I., Ecija, D., Auwarter, W. & Barth, J. V. Controlled manipulation of electronic properties of a double-decker DyPc2 molecule at the surface. Phys. – gadolinium-coordinated supramolecules by low-temperature scanning Chem. Chem. Phys. 17, 27019 27026 (2015). tunneling microscopy. Nano Lett. 14, 1369–1373 (2014). 54. Yajie, Z. et al. Detection and manipulation of charge states for double-decker ﬁ – 22. Urgel, J. I. et al. Five-vertex lanthanide coordination on surfaces: a route to DyPc2 molecules on ultrathin CuO lms. ACS Nano 12, 2991 2997 (2018). sophisticated nanoarchitectures and tessellations. J. Phys. Chem. C 118, 55. Horcas, I. et al. WSXM: a software for scanning probe microscopy and a tool 12908–12915 (2014). for nanotechnology. Rev. Sci. Instrum. 78, 013705 (2007). – 23. Urgel, J. I. et al. Surface-supported robust 2D lanthanide-carboxylate 56. Blöchl, P. E. Projector augmented-wave method. Phys. Rev. B 50, 17953 17979 coordination networks. Small 11, 6358–6364 (2015). (1994). 24. Fan, Q. et al. Template-controlled on-surface synthesis of a lanthanide 57. Kresse, G. & Joubert, D. From ultrasoft pseudopotentials to the projector – supernaphthalocyanine and its open-chain polycyanine counterpart. Nat. augmented-wave method. Phys. Rev. B 59, 1758 1775 (1999). ﬁ Commun. 10, 5029 (2019). 58. Kresse, G. & Furthmuller, J. Ef cient iterative schemes for ab initio total- 25. Classen, T. et al. Templated growth of metal-organic coordination chains at energy calculations using a plane-wave basis set. Phys. Rev. B 54, 11169 (1996). surfaces. Angew. Chem. 44, 6142–6145 (2005). 59. Klimes, J., Bowler, D. R. & Michaelides, A. Chemical accuracy for the van der 26. Wang, W. et al. Inspecting metal-coordination-induced perturbation of Waals density functional. J. Phys. Condens. Matter 22, 022201 (2010). molecular ligand orbitals at a submolecular resolution. J. Phys. Chem. Lett. 1, 60. Lee, K., Murray, É. D., Kong, L., Lundqvist, B. I. & Langreth, D. C. Higher- 2295–2298 (2010). accuracy van der Waals density functional. Phys. Rev. B 82, 081101 (2010). š 27. Wang, W., Wang, S., Hong, Y., Tang, B. Z. & Lin, N. Selective supramolecular 61. Klime , J., Bowler, D. R. & Michaelides, A. Van der Waals density functionals assembly of multifunctional ligands on a Cu(111) surface: metallacycles, applied to solids. Phys. Rev. B 83, 195131 (2011). propeller trimers and linear chains. Chem. Commun. 47, 10073–10075 62. Hafer, J. Ab-initio simulations of materials using VASP: density-functional – (2011). theory and beyond. J. Comput. Chem. 29, 2044 2078 (2008). 28. Knecht, P. et al. The self-assembly and metal adatom coordination of a linear – bis-tetrazole ligand on Ag(111). Chem. Commun. 54, 10072 10075 (2018). Acknowledgements 29. Krull, C. et al. Iron-based trinuclear metal-organic nanostructures on a surface This work was supported by the Ministry of Science and Technology (2018YFA0306003, with local charge accumulation. Nat. Commun. 9, 3211 (2018). 2017YFA0205003) and National Natural Science Foundation of China (22001017, 30. Yan, L. et al. Stabilizing and organizing Bi Cu and Bi Cu nanoclusters in 3 4 7 12 21972002, and 21991132). DFT calculations were carried out on TianHe-1A at National two-dimensional metal-organic networks. Angew. Chem. Int. Ed. 57, Supercomputer Center in Tianjin and supported by high-performance computing plat- 4617–4621 (2018). form of Peking University.
NATURE COMMUNICATIONS | (2021) 12:1619 | https://doi.org/10.1038/s41467-021-21911-z | www.nature.com/naturecommunications 9 ARTICLE NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-021-21911-z
Author contributions Reprints and permission information is available at http://www.nature.com/reprints Y.W. designed the experiment; J. Liu, Z.X., Q.X., and R.L. conducted the STM experi- ments; J. Li., R.S., H.T., and B.W. carried out DFT calculations; X.Z,. T.W., and M.Z. Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in conducted the XPS experiments; J. Liu, Q.X., S.G., Z.S., B.W., S.H., and Y. W. analyzed published maps and institutional afﬁliations. the data; S.G., Z.S., B.W., and S.H. participated in manuscript writing; J. Liu, Q.X., and Y.W. wrote the manuscript. All authors discussed the results and commented on the manuscript. Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, Competing interests adaptation, distribution and reproduction in any medium or format, as long as you give The authors declare no competing interests. appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party ’ Additional information material in this article are included in the article s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the Supplementary information The online version contains supplementary material article’s Creative Commons license and your intended use is not permitted by statutory available at https://doi.org/10.1038/s41467-021-21911-z. regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/ Correspondence and requests for materials should be addressed to Y.W. licenses/by/4.0/. Peer review information Nature Communications thanks J. Michael Gottfried and the other, anonymous, reviewer(s) for their contribution to the peer review of this work. Peer © The Author(s) 2021 reviewer reports are available.
10 NATURE COMMUNICATIONS | (2021) 12:1619 | https://doi.org/10.1038/s41467-021-21911-z | www.nature.com/naturecommunications